Analysis of high loss viscoelastic composites


 Kory Fleming
 1 years ago
 Views:
Transcription
1 Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science Program and Rheology Research Center University of WisconsinMadison 47 Engineering Research Building 500 Engineering Drive, Madison, WI adapted from J. Materials Science, 28, , (993). Address correspondence to R. Lakes Synopsis A theoretical study of viscoelastic properties of composites is presented with the aim of identifying structures which give rise to a combination of high stiffness and high loss tangent. Laminates with Voigt and Reuss structure, as well as composite materials attaining the HashinShtrikman bounds on stiffness were evaluated via the correspondence principle. Similarly, viscoelastic properties of composites containing spherical or platelet inclusions were explored. Reuss laminates and platelet filled materials composed of a stiff, low loss phase and a compliant high loss phase were found to exhibit high stiffness combined with high loss tangent. INTRODUCTION Viscoelastic materials can be of use in the damping of mechanical vibration and in the absorption of sound. The loss tangent, or tangent of the phase angle δ between stress and strain in sinusoidal loading, is a useful measure of material damping. Most materials used in structural applications, however, have small loss tangents. Conversely, materials with high loss tangents tend to be compliant, hence not of structural interest. Fig. contains a stiffnessloss map (plot of the absolute value of the dynamic modulus vs loss tangent) for some representative materials. Compliant, lossy materials are used as layers over stiff materials in various applications; nevertheless a stiff material with high loss would be of use in structural damping of noise and vibration. We consider in this article the possibility of making composite microstructures providing high stiffness and high loss. A possible avenue for making high loss composites is to make use of nonaffine deformation. This is in contrast to affine deformation in which the particles in the solid move in a way corresponding to a uniform strain plus a rotation in a continuum. The negative Poisson's ratio materials developed by Lakes (987) exhibit this property in that the foam cells unfold during deformation (Lakes, 99; Chen and Lakes, 99). Non
2 affine deformation can result in high viscoelastic loss in a composite if the phase which has the highest loss experiences a larger strain than does the composite as a whole. Elastic properties of multiphase composite materials have been studied extensively. Of these studies, the ones most relevant to the present work are those dealing with bounds on the elastic behavior and predicted properties of composites of relatively simple structure. The upper and lower bounds of stiffness of two phase and many phase composite materials have been obtained in terms of volume fraction of constituents (Hashin, 962; Hashin and Shtrikman, 963). Bounds and expressions for the effective elastic moduli of materials reinforced by parallel hollow circular fibers in hexagonal or random arrays have also been derived by a variational method (Hashin, 962). Furthermore, bounds on three independent effective elastic moduli of an nphase fiber reinforced composite of arbitrary transverse phase geometry, plane strain bulk modulus, transverse shear modulus and shear modulus in plane parallel to fibers, have been derived in terms of phase volume fractions(hashin, 965a). For viscoelastic heterogeneous media of several discrete linear viscoelastic phases with known stressstrain relations, it was shown that the effective relaxation and creep functions could be obtained by the correspondence principle of the theory of linear viscoelasticity (Hashin, 965b). In some cases explicit results in terms of general linear viscoelastic matrix properties was given, and thus permitting direct use of experimental information (Hashin, 966). In a review by Ahmed and Jones (990) of particulate reinforcement theories for polymer composites, it was concluded that the macroscopic behavior was affected by the size, shape, distribution, and interfacial adhesion of the inclusions. This article makes use of some of these results for elastic composites to explore accessible regions of the stiffnessloss maps of the materials. ELASTIC AND VISCOELASTIC PROPERTIES OF COMPOSITES For the simplest case of a twophase composite, the Voigt and Reuss composites described below represent rigorous upper and lower bounds on the Young's modulus for a given volume fraction of one phase. The HashinShtrikman composites represent upper and lower bounds for isotropic elastic composites. Viscoelastic composites containing spherical or platelet inclusions are also considered. Results obtained via the correspondence principle are plotted as "stiffnessloss maps" in the subsequent section. Voigt composite Let phase be stiff; let phase 2 be high loss. The geometry of the Voigt model structure is shown in Figure 2. The composite can contain laminations as shown in Figure (a) or it can be made of continuous fibers in Figure (b); in either case the strain in each phase is the same. For an elastic material with one of these structures, the Voigt relation is E c = E V + E 2 V 2, in which E c, E and E 2 refer to the Young's modulus of the composite, phase and phase 2, and V and V 2 refer to the volume fraction of phase and phase 2 with V +V 2 =. The Voigt relation for the stiffness of an elastic composite is obtained by recognizing that for the given geometry, the strain in each phase is the same; the forces in each phase are additive. By the correspondence principle (Hashin, 970, Christensen, 980), the elastic relation can be converted to a steady state harmonic viscoelastic relation by replacing the Young's moduli E by E * (iω) or E *, in which ω is the angular frequency of the harmonic loading. This procedure gives E c * = E * V + E 2 * V2 ()
3 with E * = E' + i E" and loss tangent tan δ = E"/E'. Taking the ratio of real and imaginary parts, we obtain the loss tangent of the composite tan δ c = E c "/E c '. V tanδ + V E 2 ' 2 tanδ 2 tan δ c = E ' V + E 2 ' E ' V 2 Reuss composite The geometry of the Reuss model structure is shown in Figure (c); each phase experiences the same stress. For elastic materials, /E c = V /E + V 2 /E 2. Again using the correspondence principle, the viscoelastic relation is obtained as E c * = V E * + V 2 E 2 * (3) Again separating the real and imaginary parts of E c *, the loss tangent of the composite tan δ c is obtained: E (tanδ +tanδ 2 )[V +V ' 2 E tan δ c = 2 ' ](tanδ tanδ 2 )[V tanδ 2 +V 2 tanδ E ' E 2 ' ] E (tanδ tanδ 2 )[V +V ' 2 E 2 ' ]+(tanδ +tanδ 2 )[V tanδ 2 +V 2 tanδ E ' (4) E 2 ' ] (2) HashinShtrikman composite: arbitrary twophase geometry Allowing for 'arbitrary' phase geometry, the upper and lower bounds on the elastic moduli as a function of composition have been developed using variational principles. The lower bound for the shear modulus G L of the composite was given as (Hashin and Shtrikman, 963) V G L = G 2 + G G + 6(K 2 +2G 2 )V (5) 2 2 5(3K 2 +4G 2 )G 2 in which K, G and V, and G 2 and V 2 are the bulk modulus, shear modulus and volume fraction of phases, and 2, respectively. Here G >G 2, so that G L represents the lower bound on the shear modulus. Interchanging the numbers and 2 in Equation(5) results in the upper bound G U for the shear modulus. As for viscoelastic materials, we again apply the correspondence principle. The complex viscoelastic shear moduli of the composite G L * and G U * are obtained as G L * = G2 * V + G * G2 * + 6(K 2 * +2G2 * )V2 5(3K 2 * +4G2 * )G2 * and (6)
4 G U * = G * V + 2 G 2 * G * + 6(K * +2G * (7) )V 5(3K * +4G * )G * In these cases the loss tangent is more complicated to write explicitly, so it is more expedient to graphically display computed numerical values. Hashin transversely isotropic fiber reinforced composites This case is of interest since it allows more than two phases, a situation applicable to the analysis of experimental results in a companion article. For two phases the results are almost identical to the arbitrary phase geometry case considered above. The shear modulus of elastic multiphase transversely isotropic fiber reinforced composites of arbitrary transverse phase geometry, can be bounded from below and above in terms of phase moduli and phase volume fractions. The lower and upper bounds on the shear modulus m ( ) and m (+) were given for elastic composites (Hashin, 965a) as and m () = G + 2G (K +G ) K +2G r=n {[ r=2 (G r G )V r G +K G /(K +2G )]  }  (8) m (+) = G n + 2G n (K n +G n ) K n +2G n {[ r=n (G r G n )V r G r +K n G n /(K n +2G n )]  }  (9) r= in which n is the number of the phases, G and K are the shear and bulk moduli of the most compliant phase, G n and K n are the shear and bulk moduli of the stiffest phase. r is a free index representing the phase number; phases are numbered in order of increasing stiffness. On the basis of the correspondence principle, corresponding results for the complex shear modulus (not necessarily bounds) of the composites are again obtained by replacing m(), m(+), G, K, G r and G n by G L *, GU *, G *, K *, Gr * and G n * in Equations(8) and (9), respectively. The loss tangent again is complicated to write explicitly, so it is graphically displayed using computed numerical values. Spherical particulate inclusions For a small volume fraction V =  V 2 of spherical elastic inclusions in a continuous phase of another elastic material, the shear modulus of the composite G c was given as(christensen, 979) G c G =  5(ν ) (  G 2 G )V 2 75ν +2(45ν ) G 2 G (0) in which ν is the Poisson's ratio of phase, and phase and phase 2 represent the matrix material and the inclusion material respectively. Using the correspondence principle again and assuming there is no relaxation in Poisson's ratio, Equation(0) becomes
5 G c * = G * 5(ν  ) (G *  G 2 * )V 2 75ν +2(45ν ) G 2 * () G * for the complex shear modulus of the composite material. The loss tangent again is complicated to write explicitly, so it is graphically displayed using computed numerical values. Platelet inclusions For a dilute suspension of platelet elastic inclusions of phase 2 in a matrix of phase, the shear modulus of the composite G c was given as(christensen, 979) G c = G + V 2 (G 2 G ) 5 [ 9K 2 +4(G +2G 2 ) K G 3 G G 2 ] (2) 2 Again, using the correspondence principle, Equation(2) becomes G c * = G * + V 2 (G 2 * G * ) 5 [ 9K 2 * +4(G * +2G2 * ) G K 2 * G 2 * + 6 * G 2 *] (3) for the complex shear modulus of the composite materials. As for procedure, we remark that although Equations (5) to (3) were developed for the shear modulus of the composite, the shear moduli G * were replaced by the Young's moduli E * in the figures for comparison with Fig.. The Voigt and Reuss relations given by Equations () and (3) apply to G * as well as to E *. The actual relationship between E * and G * and the properties of the constituents of a composite is simple only for certain phase geometries. For example, for some common phase geometries, a Poisson's ratio of 0.3 for each phase gives a Poisson's ratio close to or equal to 0.3 for the composite. However for some phase geometries, a constituent Poisson's ratio of 0.3 can give rise to a negative Poisson's ratio in cellular solids with one phase void (Lakes, 987) or in unusual laminates (Milton, in press). The calculations are on the basis that V +V 2 = except that V +V 2 =0.8 for the multiphase Hashin elastic bound, for which 20% void by volume fraction is assumed to be contained as a third phase in the composite. RESULTS AND DISCUSSION Results are plotted as stiffnessloss maps (plots of E * vs tan δ) as shown in Figures 24 below. Figure 2 shows predicted properties of composites containing phases which differ greatly in properties. Steel is considered as phase, with E * =200 GPa, tan δ = 0.00 and and a viscoelastic elastomer as phase 2, with E 2 * =0.020 GPa, tan δ2 =.0. The graph was enlarged in the vicinity of 00% phase and shown in Figure 3 for clarity. A small volume fraction of phase 2 results in a large increase in loss with little reduction in stiffness so that the Reuss structure permits higher losses than the Voigt structure. However, in the Reuss structure each phase carries the full stress, so that a composite of this type will not be strong if, as is usual, the soft phase 2 is weak. As for 'bounds' on the properties, the curves for the Voigt and Reuss composites enclose a region in the stiffnessloss map, as do the curves for the upper and lower Hashin Shtrikman composites. It is tempting to think of these curves as 'bounds' on the viscoelastic behavior, however such a surmise has not been proven. They represent extremes of composites which can be fabricated, however we do not yet know if they
6 represent true bounds. Roscoe (969) has mathematically established bounds for the real and imaginary parts E ' and E '' of the complex modulus of composites and has shown them to be equivalent to the Voigt and Reuss relations. Therefore the stiffness, expressed as E * of the composite is bounded from above by the Voigt limit and cannot exceed the stiffness of the stiff phase. This is not quite the same as establishing bounds for a stiffnessloss map since it is not obvious whether a maximum in tan δ = E"/E' could be obtained simultaneously with a maximum in E'. In particular, we can construct tan δ c = E" voigt /E' reuss > E" reuss /E' reuss and be within the bounds of Roscoe. We do not yet know if such a composite is physically realizable. In the stiffnessloss map, the lower and upper twophase Hashin composites behave similarly to the Voigt and Reuss composites, respectively. This is in contrast to the usual plots of elastic stiffness vs volume fraction, in which the Hashin bounds can differ greatly from the Voigt/Reuss ones. As for the physical attainment of the Voigt and Reuss composites, simple laminates can be made as in Fig., but these are anisotropic. Isotropic composites which attain the Voigt or Reuss moduli are not considered to be attainable. Isotropic polycrystals attaining the Voigt or Reuss bounds for the bulk modulus are also possible (Avellaneda and Milton, 989) at the expense of some added structural complexity. For the threephase Hashin structure with 20% void content in the composite, the lower curve reduces to zero and is not shown in the graph; the upper bound lies close to the Voigt curve with 20% to 40% lower stiffness as shown in Fig. 2. The composite containing soft spherical inclusions is also found to behave similarly to the Voigt composite in that a small volume fraction of soft, viscoelastic material has a minimal effect on the loss tangent, though it does reduce the stiffness. As for the composite containing soft platelet inclusions, it is found that the results are similar to those of the Reuss structure. A small volume fraction of platelet inclusions as phase 2 results in a very large increase in loss tangent without any significant reduction in the stiffness. However, soft platelets resemble pennyshaped cracks in the matrix, so that such a composite would be weaker than the matrix, particularly if the matrix were brittle. Figure 4 shows predicted properties of composites containing phases which do not differ so much in properties as steel and viscoelastic elastomers. Copper as phase, with E * =7 GPa, tanδ = and indium as phase 2, with E 2 * =0.8 GPa, tanδ2 =0.025 (at khz) were used for this investigation. Observe that the shape of this stiffnessloss map differs from the case of the polymermetal composite. The implication of this difference in shape is as follows. If the constituents differ by orders of magnitude in stiffness and loss, then the Reuss and platelet composites are orders of magnitude superior to the Voigt and spherical inclusion composites in achieving high stiffness and high loss. If the constituents do not differ so much in their properties, their composites of various structures do not differ as much either. Composites containing a stiff, low loss material (such as a metal) and a small amount of compliant, high loss material can exhibit a stiffness close to that of the metal, as well as high loss superior to that of a metalmetal composite. An interesting aspect of the Reuss and platelet composites which give the highest loss (for given stiffness) is that they exhibit highly nonuniform strain fields. The strain in the soft, lossy phase is much larger than the strain in the stiff phase. This is in contrast to the Voigt composite in which the strain in each phase is the same. The reentrant foams (Chen and Lakes, 989, in press) with a negative Poisson's ratio also exhibit nonaffine deformation of a more complex nature in that the foam cells unfold as the foam is deformed. CONCLUSIONS
7 . In a stiffnessloss map, the upper and lower twophase Hashin composites behave similarly to the Voigt and Reuss composites, respectively. 2. Reuss laminates and platelet filled materials based on a stiff, low loss phase and a compliant high loss phase were found to exhibit high stiffness combined with high loss tangent. However, in the Reuss structure each phase carries the full stress, so that a composite of this type will not be strong if, as is usual, the compliant phase is weak. 3. A composite containing soft lossy spherical inclusions in a stiff matrix behaves similarly to the Voigt composite: low loss and a reduction in stiffness. 4. Composites containing a metal and a small amount of compliant, high loss polymer can in principle exhibit a stiffness close to that of the metal, as well as high loss. ACKNOWLEDGMENT We thank the ONR for their support of this work. We also thank the University of Iowa for a University Faculty Scholar Award to one of the authors (RSL). REFERENCES Ahmed, S., and Jones, F.R. (990), "A review of particulate reinforcement theories for polymer composites", J. Materials Sci., 25, Avellaneda, M. and Milton, G., (989) "Optimal bounds on the effective bulk modulus of polycrystals", SIAM J. Appl. Math. 49, Chen, C.P. and Lakes, R.S., (99) "Holographic study of conventional and negative Poisson's ratio metallic foams: elasticity, yield, and microdeformation", J. Materials Science 26, Chen, C.P. and Lakes, R.S., (989)"Dynamic wave dispersion and loss properties of conventional and negative Poisson's ratio polymeric cellular materials", Cellular polymers, 8, Christensen, R.M., Theory of viscoelasticity, 2nd ed., Academic Press, New York, 982. Christensen, R.M., Mechanics of composite materials, John Wiley & Sons, New York, 979. Ferry, J. D. Viscoelastic properties of Polymers, 2nd ed J. Wiley, N.Y., 979 Hashin, Z., (962) "The elastic moduli of heterogeneous materials", J. Appl. Mech., Trans. ASME, 84E, Hashin Z., and B. W. Rosen, (964),"The elastic moduli of fiberreinforced materials", J. Appl. Mech., Trans. ASME, 3, Hashin, Z., (965a),"On elastic behaviour of fibre reinforced materials of arbitrary transverse phase geometry", J. Mech. Phys. solids, 3, Hashin, Z., (965b), "Viscoelastic behavior of heterogeneous media", J. Appl. Mech., Trans. ASME, 32E,
8 Hashin, Z., (966), "Viscoelastic fiber reinforced materials", AIAA Jnl., 4, Hashin, Z., (970), "Complex moduli of viscoelastic composites: I. General theory and application to participate composites", Int. J. Solids, Structures, 6, Hashin Z., and Shtrikman, S. (963),"A variational approach to the theory of the elastic behavior of multiphase materials", J. Mech. Phys. solids,, Katz, J. L. (97),"Hard tissue as a composite material  I. Bounds on the elastic behavior", J. Biomechanics, 4, Lakes, R.S. (987),"Foam structures with a negative Poisson's ratio", Science, 235, Lakes, R.S. (99), "Deformation mechanisms of negative Poisson's ratio materials: structural aspects", J. Materials Science, 26, Lakes, R.S., Katz, J.L., and Sternstein, S.S., (979), "Viscoelastic properties of wet cortical bone: Part I, torsional and biaxial studies." Journal of Biomechanics, 2, Milton, G., (in press) "Laminates with a negative Poisson's ratio". Nielsen, I., Mechanical Properties of Polymers, Reinhold, 962. Nowick A. S. and Berry, B. S.Anelastic relaxation in crystalline solids, Academic, N.Y., 972. Roscoe, R., (969), "Bounds for the real and imaginary parts of the dynamic moduli of composite viscoelastic systems", J. Mech. Phys. Solids, 7, Shipkowitz, A.T., Chen, C.P. and Lakes, R.S., (988), "Characterization of highloss viscoelastic elastomers", Journal of Materials Science, 23, Zener, C. Elasticity and anelasticity of metals, University of Chicago Press, 948.
9 Figures 000 E(GPa) Steel Copper Aluminum Bone Polystyrene PMMA Polycarbonate.0 Hevea rubber High loss elastomer tan δ. Stiffness vs loss tangent for some representative materials at or near room temperature. Steel, Hz, after Nowick and Berry (972) Copper, 600 Hz, after Nowick and Berry (972) Polymethyl methacrylate, (PMMA), 0 Hz and khz, after Ferry (979) Bone, 00 Hz, after Lakes, Katz, Sternstein (979) Hevea rubber, 0 Hz2 khz, after Ferry (979) Polystyrene, 00 Hz, khz, after Ferry (979) Polycarbonate, 00 Hz, after Nielsen (962) Viscoelastic elastomer, 00,,000 Hz, after Shipkowitz, et. al. (988) (a) (b) (c) 2. (a) Laminated Voigt structure. (b) Fibrous Voigt structure. (c) Reuss structure.
10 0 3 Platelet Vi: % Phase Reuss V: % Platelet Vi: 0.00% 0 2 Spherical VI: 0% Hashin V: 99.9% E* ( GPa ) Voigt V: 0% Hashin, 3 phase V: 5% V2: 65% 03 Voigt V: % Hashin V: 0% 02 Spherical Vi: 45% Hashin, 3 phase V: % V2: 79% tanδ Reuss V: 99% Reuss V: 50% Phase Stiffnessloss map for composites of steel as phase and viscoelastic elastomer as phase 2. x: Voigt curve, +: Reuss curve, : twophase Hashin curve, : upper curve of threephase Hashin composite with 20% voids as one phase. o: composite with phase 2 as dilute spherical inclusions. _ : composite with phase 2 as dilute platelet inclusions.
11 0 3 Reuss V2: 0.000% E* ( GPa ) Phase Platelet Vi: 0.000% Platelet Vi: % Spherical Vi: 5% Spherical Vi: 25% Voigt V2: 25% tan δ Stiffnessloss map for composites of steel as phase and viscoelastic elastomer as phase 2; expanded plot of upper left portion of Fig. 3. x: Voigt curve, +: Reuss curve, : upper curve of threephase Hashin composite with 20% voids as one phase. o: composite with phase 2 as dilute spherical inclusions. _ : composite with phase 2 as dilute platelet inclusions.
12 0 3 Platelet Vi: 0.5% Spherical Vi: 0% Reuss V: 99% Hashin V: 97% Platelet Vi: 3% Spherical Vi: 30% E* ( GPa ) Phase 03 Voigt V: 75% Hashin, 3 phase V: 60% V2: 20% Hashin V: 50% Voigt V: 25% 02 tanδ Reuss V: 75% Phase 2 Hashin, 3 phase V: 30% V2: 50% 05. Stiffnessloss map for composites of copper as phase and indium as phase 2. x: Voigt bound, +: Reuss curve, : twophase Hashin curve, : upper curve of threephase Hashin composite with 20% voids as one phase. o: composite with phase 2 as dilute spherical inclusions. _ : composite with phase 2 as dilute platelet inclusions.
Module 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationViscoelastic Damping Characteristics of IndiumTin/SiC Particulate Composites
Viscoelastic Damping Characteristics of IndiumTin/SiC Particulate Composites HyungJoo Kim, Colby C. Swan Ctr. for ComputerAided Design, Univ. of Iowa Roderic Lakes Engineering Physics, Univ. of Wisconsin
More informationH Kalathur 1, 2 1, 2,3. , R S Lakes. 3
Column dampers with negative stiffness: high damping at small amplitude adapted from Kalathur, H., Lakes, R. S., Column dampers with negative stiffness: high damping at small amplitude, Smart Materials
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationDesign of a fastener based on negative Poisson's ratio foam adapted from
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205212 (1991).
More informationPiezoelectric composite lattices with high sensitivity
Piezoelectric composite lattices with high sensitivity Roderic Lakes Department of Engineering Physics, Engineering Mechanics Program, Department of Materials Science, Rheology Research Center, University
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationMcMAT 2007 Micromechanics of Materials Austin, Texas, June 3 7, 2007
McMAT 2007 Micromechanics of Materials Austin, Texas, June 3 7, 2007 RANDOM POLYCRYSTALS OF GRAINS WITH CRACKS: MODEL OF ELASTIC BEHAVIOR FOR FRACTURED SYSTEMS James G. Berryman Earth Sciences Division
More informationEVALUATION OF EFFECTIVE MECHANICAL PROPERTIES OF COMPLEX MULTIPHASE MATERIALS WITH FINITE ELEMENT METHOD
U.P.B. Sci. Bull., Series D, Vol. 79, Iss. 3, 2017 ISSN 14542358 EVALUATION OF EFFECTIVE MECHANICAL PROPERTIES OF COMPLEX MULTIPHASE MATERIALS WITH FINITE ELEMENT METHOD Mohamed said BOUTAANI 1, Salah
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationMSE 383, Unit 33. Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept.
Dynamic Mechanical Behavior MSE 383, Unit 33 Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept. Scope Why DMA & TTS? DMA Dynamic Mechanical Behavior (DMA) Superposition Principles
More informationDeformation of Polymers. Version 2.1. Boban Tanovic, MATTER David Dunning, University of North London
Deformation of Polymers Version 2.1 Boban Tanovic, MATTER David Dunning, University of North London Assumed Preknowledge It is assumed that the user is familiar with the terms elasticity, stress, strain,
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationLoss Amplification Effect in Multiphase Materials with Viscoelastic Interfaces
Loss Amplification Effect in Multiphase Materials with Viscoelastic Interfaces Andrei A. Gusev Institute of Polymers, Department of Materials, ETHZürich, Switzerland Outlook Lamellar morphology systems
More informationAbvanced Lab Course. DynamicalMechanical Analysis (DMA) of Polymers
Abvanced Lab Course DynamicalMechanical Analysis (DMA) of Polymers M211 As od: 9.4.213 Aim: Determination of the mechanical properties of a typical polymer under alternating load in the elastic range
More informationDynamic Mechanical Analysis (DMA) of Polymers by Oscillatory Indentation
Dynamic Mechanical Analysis (DMA) of Polymers by Oscillatory Indentation By Jennifer Hay, Nanomechanics, Inc. Abstract This application note teaches the theory and practice of measuring the complex modulus
More informationA direct evaluation of the Fabric Tensor in anisotropic porous media
A direct evaluation of the Fabric Tensor in anisotropic porous media Maria Cristina Pernice 1, Luciano Nunziante 1, Massimiliano Fraldi 1,2 1 Department of Structural Engineering, University of Naples
More informationForced Response of Plate with Viscoelastic Auxetic Dampers
Vibrations in Physical Systems 2018, 29, 2018003 (1 of 9) Abstract Forced Response of Plate with Viscoelastic Auxetic Dampers Tomasz STREK Poznan University of Technology, Institute of Applied Mechanics
More informationContinuum Modeling Techniques to Determine Mechanical Properties of Nanocomposites
International OPEN ACCESS Journal Of Modern Engineering Research (IJMER) Continuum Modeling Techniques to Determine Mechanical Properties of Nanocomposites Sonali Gholap 1, Dr. Dhananjay R. Panchagade
More informationNONLINEAR MECHANICS OF VISCOELASTIC LAYERED COMPOSITES. A Thesis Presented to The Academic Faculty. Kashyap Alur
NONLINEAR MECHANICS OF VISCOELASTIC LAYERED COMPOSITES A Thesis Presented to The Academic Faculty y Kashyap Alur In Partial Fulfillment Of the Requirements for the Degree Master of Science in Mechanical
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationSupplementary figures
Supplementary figures Supplementary figure 1: The fang model (longitudinal section) used for the stiffness analysis. The base of the fang is considered fixed (i.e. zero displacement constraint) and the
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationMeasurement Engineering Group, Paderborn University, Warburger Straße 100, Paderborn, Germany
Nadine Feldmann 1, Fabian Bause 1, Bernd Henning 1 1 Measurement Engineering Group, Paderborn University, Warburger Straße 100, 33098 Paderborn, Germany feldmann@emt.unipaderborn.de Abstract The present
More informationNumerical evaluation of effective material properties of randomly distributed short cylindrical fibre composites
Computational Materials Science 39 (2007) 198 204 www.elsevier.com/locate/commatsci Numerical evaluation of effective material properties of randomly distributed short cylindrical fibre composites S. Kari
More informationTesting Elastomers and Plastics for Marc Material Models
Testing Elastomers and Plastics for Marc Material Models Presented by: Kurt Miller Axel Products, Inc. axelproducts.com We Measure Structural Properties Stress Strain TimeTemperature Test Combinations
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationCHAPTER 4 MODELING OF MECHANICAL PROPERTIES OF POLYMER COMPOSITES
CHAPTER 4 MODELING OF MECHANICAL PROPERTIES OF POLYMER COMPOSITES 4. Introduction Fillers added to polymer matrices as additives are generally intended for decreasing the cost (by increase in bulk) of
More informationFinite Element of Composite Materials with Partial Debonding along Boundary. Kohei HIGUCHI, Tetsuo IWAKUMA
Vol. 8 (2005 8 ) Finite Element of Composite aterials with Partial Debonding along Boundary Kohei HIGUCHI, Tetsuo IWAKUA JFE PhD 9808579 6606 Damages in composite materials are mostly governed by interfacial
More informationA micromechanical model for effective elastic properties of particulate composites with imperfect interfacial bonds
International Journal of Solids and Structures 42 (2005) 4179 4191 www.elsevier.com/locate/ijsolstr A micromechanical model for effective elastic properties of particulate composites with imperfect interfacial
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationAn Exact Result for the Macroscopic Response of ParticleReinforced NeoHookean Solids
Oscar LopezPamies Department of Mechanical Engineering, State University of New York, Stony Brook, NY 9 email: oscar.lopezpamies@sunysb.edu An Exact Result for the Macroscopic Response of ParticleReinforced
More informationFrancisco Paulo Lépore Neto. Marcelo Braga dos Santos. Introduction 1. Nomenclature. Experimental Apparatus and Formulation
Francisco Paulo Lépore Neto and Marcelo Braga dos Santos Francisco Paulo Lépore Neto fplepore@mecanica.ufu.br Federal University of Uberlandia School of Mechanical Engineering 38408902 Uberlandia, MG,
More informationXI. NANOMECHANICS OF GRAPHENE
XI. NANOMECHANICS OF GRAPHENE Carbon is an element of extraordinary properties. The carboncarbon bond possesses large magnitude cohesive strength through its covalent bonds. Elemental carbon appears in
More informationCHARACTERIZATION OF POLYMERS BY MEANS OF A STANDARD VISCOELASTIC MODEL AND FRACTIONAL DERIVATE CALCULUS
International Journal of Polymeric Materials, 53:633 644, 2004 Copyright # Taylor & Francis Inc. ISSN: 00914037 print=15435253 online DOI: 10.1080/00914030490472845 CHARACTERIZATION OF POLYMERS BY MEANS
More informationProperties of a chiral honeycomb with a Poisson's ratio 1
Properties of a chiral honeycomb with a Poisson's ratio 1 D. Prall, R. S. Lakes Int. J. of Mechanical Sciences, 39, 305314, (1996). Abstract A theoretical and experimental investigation is conducted
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationThe Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials under Kinematic Harmonic Loading
Mechanics and Mechanical Engineering Vol. 21, No. 1 (2017) 157 170 c Lodz University of Technology The Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials
More informationHolographic study of conventional and negative Poisson's ratio metallic foams: elasticity, yield, and microdeformation by
Holographic study of conventional and negative Poisson's ratio metallic foams: elasticity, yield, and microdeformation by 1 C. P. Chen and R. S. Lakes J. Materials Science, 26, 53975402 (1991) 2 Abstract
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationChapter 5: Modeling Bone as a TwoPhase Composite
Chapter 5: Modeling Bone as a TwoPhase Composite Fundamental finite element models are constructed for mineralized tissues at the ultrastructual lengthscale to examine the basic composite mechanics and
More informationD Y N A M I C M E C H A N I C A L A N A L Y S I S A N D I T S A D V A N T A G E S O V E R D E F L E C T I O N T E M P E R A T U R E U N D E R L O A D
D Y N A M I C M E C H A N I C A L A N A L Y S I S A N D I T S A D V A N T A G E S O V E R D E F L E C T I O N T E M P E R A T U R E U N D E R L O A D Sujan E. Bin Wadud TA Instruments 9 Lukens Drive, New
More informationA GENERALIZED CROSSPROPERTY RELATION BETWEEN THE ELASTIC MODULI AND CONDUCTIVITY OF ISOTROPIC POROUS MATERIALS WITH SPHEROIDAL PORES
journal webpage: www.ceramicssilikaty.cz CeramicsSilikáty 61 (1, 7480 (017 doi: 10.13168/cs.016.0063 A GENERALIZED CROSSPROPERTY RELATION BETWEEN THE ELASTIC MODULI AND CONDUCTIVITY OF ISOTROPIC POROUS
More informationMODELING AND FEM ANALYSIS OF DYNAMIC PROPERTIES OF THERMALLY OPTIMAL COMPOSITE MATERIALS
11th World Congress on Computational Mechanics (WCCM XI) 5th European Conference on Computational Mechanics (ECCM V) 6th European Conference on Computational Fluid Dynamics (ECFD VI) E. Oñate, J. Oliver
More informationMechanical Properties
Mechanical Properties Elastic deformation Plastic deformation Fracture I. Elastic Deformation S s u s y e u e T I II III e For a typical ductile metal: I. Elastic deformation II. Stable plastic deformation
More informationComposite angle ply laminates and netting analysis
10.1098/rspa.2002.1066 FirstCite epublishing Composite angle ply laminates and netting analysis By J. T. Evans and A. G. Gibson School of Mechanical and Systems Engineering, University of Newcastle upon
More informationInternational Journal of Engineering Science
International Journal of Engineering Science 49 (2011) 322 332 Contents lists available at ScienceDirect International Journal of Engineering Science ournal homepage: www.elsevier.com/locate/iengsci On
More informationVISCOELASTIC PROPERTIES OF POLYMERS
VISCOELASTIC PROPERTIES OF POLYMERS John D. Ferry Professor of Chemistry University of Wisconsin THIRD EDITION JOHN WILEY & SONS New York Chichester Brisbane Toronto Singapore Contents 1. The Nature of
More informationMechanical Properties of Polymers. Scope. MSE 383, Unit 31. Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept.
Mechanical Properties of Polymers Scope MSE 383, Unit 31 Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept. Structure  mechanical properties relations Timedependent mechanical
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More informationCHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement
CHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement Mark Hughes 19 th September 2016 Outline Fibre architecture Volume fraction and the rule of mixtures Principle
More informationStability of Cosserat solids: size effects, ellipticity and waves
Stability of Cosserat solids: size effects, ellipticity and waves Roderic S. Lakes Department of Engineering Physics, Engineering Mechanics Program Department of Materials Science, Rheology Research Center,
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationRHEOLOGICAL AND MORPHOLOGICAL INFLUENCES ON THE VISCOELASTIC BEHAVIOUR OF POLYMER COMPOSITES
RHEOLOGICAL AND MORPHOLOGICAL INFLUENCES ON THE VISCOELASTIC BEHAVIOUR OF POLYMER COMPOSITES R. Gaertner 1 and 2, C. Gauthier 1, P. Franciosi 1, A. Khavandi 1 and M. Shaterzadeh 1 1 GEMPPM  UMR 5510,
More informationFrancisco Paulo Lépore Neto. Marcelo Braga dos Santos. Introduction 1. Nomenclature. Experimental Apparatus and Formulation
A Procedure for the Parametric Identification of Viscoelastic Dampers Accounting for Preload Francisco Paulo Lépore Neto fplepore@mecanica.ufu.br Federal University of Uberlândia School of Mechanical Engineering
More informationDevelopment of a code to generate randomly distributed short fiber composites to estimate mechanical properties using FEM
International Journal of Theoretical and Applied Mechanics. ISSN 09736085 Volume 12, Number 4 (2017) pp. 863872 Research India Publications http://www.ripublication.com Development of a code to generate
More informationSTUDY OF THE EFFECT OF COMPOSITE CONSTRAINED LAYERS IN VIBRATION DAMPING OF PLATES
Int. J. of Applied Mechanics and Engineering, 214, vol.19, No.1, pp.2329 DOI: 1.2478/ijame21415 Brief note STUDY OF THE EFFECT OF COMPOSITE CONSTRAINED LAYERS IN VIBRATION DAMPING OF PLATES K.S.K. SASIKUMAR
More informationTHE INFLUENCE OF INPLANE DENSITY VARIATION ON ENGINEERING PROPERTIES OF ORIENTED STRANDBOARD: A FINITE ELEMENT SIMULATION
Proceedings of McMat5: 5 Joint ASME/ASCE/SES Conference on Mechanics and Materials June 13, 5, Baton Rouge, Louisiana, USA 255 THE INFLUENCE OF INPLANE DENSITY VARIATION ON ENGINEERING PROPERTIES OF
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationSession 11: Complex Modulus of Viscoelastic Polymers
Session 11: Complex Modulus of Viscoelastic Polymers Jennifer Hay Factory Application Engineer NanoScale Sciences Division Agilent Technologies jenny.hay@agilent.com To view previous sessions: https://agilenteseminar.webex.com/agilenteseminar/onstage/g.php?p=117&t=m
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationThe effect of interfacial bonding on the damping behavior of nanocomposites
The effect of interfacial bonding on the damping behavior of nanocomposites Literature review The rapid and continuous growth in aerospace, automotive, and military applications requires special materials
More informationSupporting Information. Potential semiconducting and superconducting metastable Si 3 C. structures under pressure
Supporting Information Potential semiconducting and superconducting metastable Si 3 C structures under pressure Guoying Gao 1,3,* Xiaowei Liang, 1 Neil W. Ashcroft 2 and Roald Hoffmann 3,* 1 State Key
More informationDramatically stier elastic composite materials due to a negative stiness phase?
Journal of the Mechanics and Physics of Solids 50 (2002) 979 1009 www.elsevier.com/locate/jmps Dramatically stier elastic composite materials due to a negative stiness phase? R.S. Lakes a;b;, W.J. Drugan
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More informationMicrobuckling instability in elastomeric cellular solids
1 Microbuckling instability in elastomeric cellular solids Rosakis, P., Ruina, A., and Lakes, R. S., "Microbuckling instability in elastomeric cellular solids", J. Materials Science, 28, 46674672 (1993).
More informationASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS
ASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS Dieter H. Pahr and Helmut J. Böhm Institute of Lightweight Design and Structural
More informationADVANCES IN NEGATIVE POISSON'S RATIO MATERIALS. Roderic Lakes adapted from Advanced Materials, 5, , (1993). Diagrams at bottom.
1 ADVANCES IN NEGATIVE POISSON'S RATIO MATERIALS Roderic Lakes adapted from Advanced Materials, 5, 293296, (1993). Diagrams at bottom. 1. Introduction Poisson's ratio of a solid is defined as the lateral
More informationCompeting Effect of Pore Fluid and Texture  Case Study
Competing Effect of Pore Fluid and Texture  Case Study Depth (m) Sw Sxo. m Poisson's Ratio.. GOC.1 5 7 8 9 PImpedance OWC 15 GR.. RHOB.5 1 Saturation...5. 1. 1.5 Vs (km/s).. Poisson's Ratio 5 7 PImpedance
More informationMechanical Properties of Fiber Reinforced Composites Using Buckminster Fullerene Reinforcement
IJRMET Vo l. 4, Is s u e Sp l  1, No v 2013 Ap r i l 2014 ISSN : 22495762 (Online ISSN : 22495770 (Print Mechanical Properties of Fiber Reinforced Composites Using Buckminster Fullerene Reinforcement
More informationDynamic Finite Element Modeling of Elastomers
Dynamic Finite Element Modeling of Elastomers Jörgen S. Bergström, Ph.D. Veryst Engineering, LLC, 47A Kearney Rd, Needham, MA 02494 Abstract: In many applications, elastomers are used as a loadcarrying
More informationTensile stress strain curves for different materials. Shows in figure below
Tensile stress strain curves for different materials. Shows in figure below Furthermore, the modulus of elasticity of several materials effected by increasing temperature, as is shown in Figure Asst. Lecturer
More informationNegative incremental bulk modulus in foams
Philosophical Magazine Letters, Vol. 86, No., October 6, 65 659 Negative incremental bulk modulus in foams B. MOOREy, T. JAGLINSKIz, D. S. STONEyz and R. S. LAKES*zx{ ydepartment of Materials Science and
More informationDepartment of Mechanical Engineering, National Institute of Technology Rourkela, Rourkela , India
Composites, Article ID 629175, 12 pages http://dx.doi.org/10.1155/2014/629175 Research Article Effect of Fiber Geometry and Representative Volume Element on Elastic and Thermal Properties of Unidirectional
More informationFinal Project: Indentation Simulation Mohak Patel ENGN2340 Fall 13
Final Project: Indentation Simulation Mohak Patel ENGN2340 Fall 13 Aim The project requires a simulation of rigid spherical indenter indenting into a flat block of viscoelastic material. The results from
More informationChoi, J. B. and Lakes, R. S., "Nonlinear properties of polymer cellular materials with a negative Poisson's. ratio",
1 Choi, J. B. and Lakes, R. S., "Nonlinear properties of polymer cellular materials with a negative Poisson's ratio", J. Materials Science, 27, 46784684 (1992). Cover issue. ABSTRACT Negative Poisson's
More informationSound Propagation through Media. Nachiketa Tiwari Indian Institute of Technology Kanpur
Sound Propagation through Media Nachiketa Tiwari Indian Institute of Technology Kanpur LECTURE13 WAVE PROPAGATION IN SOLIDS Longitudinal Vibrations In Thin Plates Unlike 3D solids, thin plates have surfaces
More informationFINITE ELEMENT APPROACHES TO MESOSCOPIC MATERIALS MODELING
FINITE ELEMENT APPROACHES TO MESOSCOPIC MATERIALS MODELING Andrei A. Gusev Institute of Polymers, Department of Materials, ETHZürich, Switzerland Outlook Generic finite element approach (PALMYRA) Random
More information2.1 Strain energy functions for incompressible materials
Chapter 2 Strain energy functions The aims of constitutive theories are to develop mathematical models for representing the real behavior of matter, to determine the material response and in general, to
More informationNanoindentation of Fibrous Composite Microstructures: Experimentation and Finite Element Investigation. Mark Hardiman
Nanoindentation of Fibrous Composite Microstructures: Experimentation and Finite Element Investigation Mark Hardiman Materials and Surface Science Institute (MSSI), Department of Mechanical and Aeronautical
More informationModule 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus
Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the
More informationComputational studies on highstiffness, highdamping SiC InSn particulate reinforced composites
International Journal of Solids and Structures 39 (2002) 5799 5812 www.elsevier.com/locate/ijsolstr Computational studies on highstiffness, highdamping SiC InSn particulate reinforced composites Hyung
More informationViscoelastic Properties of Foamed Thermoplastic Vulcanizates and their Dependence on Void Fraction
Viscoelastic Properties of Foamed Thermoplastic Vulcaniates and their Dependence on Void Fraction Viscoelastic Properties of Foamed Thermoplastic Vulcaniates and their Dependence on Void Fraction Junhong
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationEvaluation of Effective Elastic Moduli Using Micromechanics
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Evaluation of Effective Elastic Moduli Using Micromechanics To cite this article: Misba Mehdi Mrs. et al 2018 IOP Conf. Ser.:
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationNondestructive and Destructive Testing of Reinforced Polymeric Materials
Copyright 2012 Tech Science Press SL, vol.8, no.2, pp.8397, 2012 Nondestructive and Destructive Testing of Reinforced Polymeric Materials E.E. Theotokoglou 1, E. Sideridis 1 Abstract: In this work a class
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationA multiscale approach for composite materials as multifield continua
Materials Science Forum Vols. 539543 (27) pp. 25512556 online at http://www.scientific.net (27) Trans Tech Publications, Switzerland A multiscale approach for composite materials as multifield continua
More informationEXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More information